SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere Nutzervereinbarung und die Datenschutzrichtlinie.
SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere unsere Datenschutzrichtlinie und die Nutzervereinbarung.
Composite integrated material of al layers with kevlar material and the specification test result
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012 Composite integrated Material of Al layers with Kevlar material and the specification test result Maria Antoine Pushparaj 1* & Zeenath Fathima 2 1. Mailam engineering college,Mailam,India 2. School of Mechanical Engineering,SRM University,Kattangulathur ,India * E-mail of the corresponding author: email@example.comAbstractWhen the Kevlar material is used for the defense purpose and for the safety purpose at the time of the war enclosurethe problem facing here is when the impact is applied at a point the material deformation occurs and at a particularpoint and the deflection will be very high so that the human who is wearing the Kevlar as the body proof experiencea heavy pain in that , concluded is we are introducing a new composite material for the Kevlar design which willconvert a point into a uniformly distributed load across the material hence by reducing the point deformationKeywords: Shear thickening fluids (STFs), transmission electron microscopy (TEM)1. Introduction Kevlar is synthesized in solution from the monomers 1,4-phenylene-diamine (para-phenylenediamine)and terephthaloyl chloride in a condensation reaction yielding hydrochloric acid as a byproduct. The resulthas liquid-crystalline behavior, and mechanical drawing orients the polymer chains in the fibersdirection. Hexamethylphosphoramide (HMPA) was the solvent initially used for the polymerization, but for safetyreasons, DuPont replaced it by a solution of N-methyl-pyrrolidone and calcium chloride. As this process waspatented by Akzo (see above) in the production of Twaron, a patent war ensued.phenylene-diamine (para-phenylenediamine) with terephthaloyl chloride yielding Kevlar.Kevlar (poly paraphenylene terephthalamide) production is expensive because of the difficulties arising from usingconcentrated sulfuric acid, needed to keep the water-insoluble polymer in solution during its synthesis and spinning.When reinforced with glass fiber, thermoplastics typically suffer a decrease in performance under humid conditionsbecause of a lack of adhesion between the glass fibre andthe resin. This challenge is key in many applicationsincluding appliance components, automotive under-the-hood and, in some case, consumer goods.2. Grades of the Kevlar 1. Kevlar K-29 – in industrial applications, such as cables, asbestos replacement, brake linings, and body/vehicle armor. 2. Kevlar K49 – high modulus used in cable and rope products. 3. Kevlar K100 – colored version of Kevlar 4. Kevlar K119 – higher-elongation, flexible and more fatigue resistant. 5. Kevlar K129 – higher tenacity for ballistic applications. 1
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012 6. Kevlar AP – has 15% higher tensile strength than K-29 7. Kevlar XP – lighter weight resin and KM2 plus fiber combination. 8. Kevlar KM2 – enhanced ballistic resistance for armor applications3. Bullet proof vestsWhen a handgun bullet strikes body armor, it is caught in a "web" of very strong fibers. These fibers absorb and disperse theimpact energy that is transmitted to the vest from the bullet, causing the bullet to deform or "mushroom." Additional energyis absorbed by each successive layer of material in the vest, until such time as the bullet has been stopped.Because the fibers work together both in the individual layer and with other layers of material in the vest, a large area of thegarment becomes involved in preventing the bullet from penetrating. This also helps in dissipating the forces which cancause no penetrating injuries (what is commonly referred to as "blunt trauma") to internal organs. Unfortunately, at this timeno material exists that would allow a vest to be constructed from a single ply of material.4. Different Materials UsedDuPont has developed law enforcement protection products for more than 25 years. Its Kevlar brand fiber, first developed in1965, was the first material identified for use in the modern generation of concealable body armor. Kevlar is a manmadeorganic fiber, with a combination of properties allowing for high strength with low weight, high chemical resistance, andhigh cut resistance. Kevlar is also flame resistant; does not melt, soften, or flow; and the fiber is unaffected by immersion inwater.Another manufacturer, Akzo Nobel, has developed various forms of its aramid fiber TWARON for body armor. Accordingto Akzo Nobel, this fiber uses 1,000 or more finely spun single filaments that act as an energy sponge, absorbing a bulletsimpact and quickly dissipating its energy through engaged and adjacent fibers. Because more filaments are used, the impactis dispersed more quickly. Akzo claims their patented Microfilament technology allows maximum energy absorption atminimum weights while enhancing comfort and flexibility.Akzo Nobel maintains that the use of TWARON in body armor significantly reduces the overall weight of the finishedproduct, thus making vests more comfortable. Akzo also contends that stitching panels made from layers of TWARON islargely unnecessary, and that the lack of stitching contributes to a lighter weight and softer feel while affording the sameprotection.Another fiber used to manufacture body armor is Dyneema. Originated in the Netherlands, Dyneema has an extremely highstrength-to-weight ratio (a 1-mm-diameter rope of Dyneema can bear up to a 240-kg load), is light enough that it can floaton water, and has high energy absorption characteristics. 2
Chemistry and Materials Research www.iiste.org ISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online) Vol 2, No.2, 2012 Areal weight: 146 g / sq.m. Weaving style: Plain Width: 1.00 meters Warp: Glass EC11-105 fiber, 54%, 7.5 ends (threads) / cm Weft: Glass EC11-105 fiber, 46%, 6.4 ends (threads) / cm 5. Technical specification of Kevlar Fibers of Kevlar consist of long molecular chains produced from poly-paraphenylene terephthalamide. The chains are highly oriented with strong interchange bonding, which results in a unique combination of properties. General properties of Kevlar®:• High Modulus• High LASE (Load At Specified Elongation)• High Tensile Strength at Low Weight• Low Elongation to Break High Modulus (Structural Rigidity)• Low Electrical Conductivity• High Chemical Resistance• Low Thermal Shrinkage• High Toughness (Work-To-Break)• Excellent Dimensional Stability• High Cut Resistance• Flame Resistant, Self-Extinguishing 6. Concepts of the composite development A previous study investigated a related, but distinct effect to improve the performance of Kevlar woven fabrics. The used fibers coated with a dry powder that exhibits dilatants properties. In their work, the fibers demonstrated an improved ability to distribute energy during ballistic impact due to the enhanced interfiles friction. The objective of this study is to investigate the ballistic properties of woven Kevlar fabrics impregnated with fluids that exhibit the shear thickening effect. At low strain rates, associated with normal motion of the wearer, the fluid will offer little impediment to fabric flexure and deformation. However, at the high strain rates associated with a ballistic impact event, the fluid will thicken and in doing so, enhance the ballistic protection of the fabric. The results of this study confirm these hypotheses, and demonstrate that the novel composite material could provide a more flexible, and less bulky, alternative to neat Kevlar fabrics. 3
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 20127. Experimental MaterialsThe colloidal silica used to produce the shear thickening fluids (STFs) for this investigation (Nissan Chemicals (MP4540))is provided as an aqueous suspension at a particle concentration of about 40 wt%. The particle size was characterized withdynamic light scattering and transmission electron microscopy (TEM). Fig. 1 shows the TEM micrographs of a dried sampleof the dispersion. The particles are bimodal in size, with a minor fraction of smaller particles. The average particle diameterwas determined to be 446 nm by dynamic light scattering. The density of the silica particles was Transmission electronmicroscopy of colloidal silica obtained from Nissan Chemicals (MP4540) at a magnification of 40,000. calculated fromdensity measurements (DMA 48 density meter (Anton Paar)) conducted on dilute samples of the dispersion. The weightfraction of silica in each solution was measured by drying in a convection oven at 180◦C for 5 h and weighing the residualdry silica. From the mass fraction, solvent density and the corresponding measured solution density, the density of the silicaparticles in solution was estimated to be 1.78 g/cc.As a means of preparing a stable, shear thickening concentrated dispersion, the aqueous medium was replaced with ethyleneglycol. Ethylene glycol was chosen as a solvent due to its low volatility and thermal stability. Additionally, the index ofrefraction of ethylene glycol is close to that of the silica particles, providing enhanced colloidal stability. Three hours ofcentrifugation at 3,900 rpm using a table top centrifuge (IEC clinical centrifuge) was performed to separate the silicaparticles from the aqueous-based supernatant. The silica sediment was then crushed using a spatula and re suspended inethylene glycol using a vortex mixer. This process was repeated 4 times in order to minimize the amount of residualaqueous supernatant present within the samples. The final weight fraction of particles in this stock solution was determinedby using a moisture analyzer (Mettle Toledo, HR73).Rheological measurements were performed primarily with a stress-controlled rheometer.To (SR-500, Rheumatics) at 25◦Cwith cone-plate geometry having a cone angle of 0.1 radian and a diameter of 25 mm. Complementary measurements wereperformed on a Rheumatics ARE Controlled strain rheometer.To minimize the effects of solvent evaporation during testing,a solvent trap was used during all remoter measurements. To remove sample loading effects, a preheat of 1 s−1 was appliedfor 60 s prior to further measurement. All measurements presented here were reproducible.7.1 Kevlar fabricThe Kevlar fabric used in all composite target constructions was plain-woven Hexcel Aramid (polyparaphenyleneterephthalamide), high performance fabric Style 706 (Kevlar KM-2, 600 denier) with an areal density of 180 g/m2.8. Target preparationEthylene glycol (surface tension = 47.7 dyne/cm) was observed to wet the Kevlar fabric. To facilitate impregnation of theSTF into the Kevlar fabric, an equal volume of ethanol surface tension (22.0 dyne/cm) was added to the original ethyleneglycol based STF. This diluted STF was observed to spontaneously impregnate the fabric. Following impregnation, thecomposite fabric was heated at 80◦C for 20 min in a convection oven to remove the ethanol from the sample. The finalcomposition of the impregnated STF is 57 vol% silica in ethylene the ethylene glycol was removed prior to imaging by 4
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012drying the sample at 200◦C for 24 h, leaving only the silica particles and Kevlar fabric. The image shows silica particlesdispersed within the yarn, 2826 demonstrating that the original STF was fully impregnated between the individual Kevlarfibers within each yarn. In addition to the STF-impregnated fabric, samples were made of fabric impregnated with neatethylene glycol.The ethylene glycol-impregnated fabric was made using the same ethanol dilution and evaporation method used for theSTF-impregnated targets is a schematic diagram of a ballistic target. Two pieces of 5.08 cm × 5.08 cm aluminum foil (1mmthickness) were used to encapsulate the targets. The Kevlar layers were cut to 4.76 cm × 4.76 cm, impregnated with varyingamounts of STF per layer (2, 4, and 8 ml) as indicated, and then assembled into the targets by stacking them to the desiredtarget configuration.To prevent leakage of STF out of the target assembly and because Kevlar is known be sensitive to moisture, heat-sealedpolyethylene film (Zip lock bags sealed using a ULINE KF-200HC heat sealer) was used to encapsulate the targets. Neitherthe aluminum foil nor the polyethylene packaging provided any measurable ballistic resistance.These targets were mounted onto a single ply of unimpregnated Kevlar, glued to a 5.08 cm diameter copper hoop (0.635 cmwire diameter) using Liquid Nails adhesive (ICI), in order to help support the target during testing. In all cases this mountedKevlar layer was immediately adjacent to the ballistic target, with the copper hoop resting inside of the target mountingframe. All subsequent descriptions of ballistic targets will list only the Kevlar layers within the aluminum foil layers, and donot include this individual backing Kevlar layer.8.1 Ballistic testsThe ballistic tests were performed using a smooth bore helium gas gun (Army Research Laboratory, MD). All tests wereperformed at room temperature. The gun was sighted on the target center and the impact velocity was adjusted toapproximately 244 m/s (800 fps). The exact impact velocity of each projectile was measured with a chronographimmediately before impacting the target. The projectile is a NATO standard fragment simulation projectile (FSP), consistingof a chisel-pointed metal cylinder of 1.1 grams (17 grains) and 0.56 cm diameter (22 caliber). A 10.16 cm × 10.16 cm × 2.54cm thick aluminum block was cut with a recessed square hole to accept the 5.08 cm square target packageThe target was held in place using light pressure from spring clips located along its edge. The mounting block was thenclamped onto a steel frame in line with the gas gun barrel. A clay witness was used to measure the depth of indentationModeling clay (Van Aken International) was packed into a 15.24 cm × 8.89 cm × 8.89 cm wooden mold, compressed with amallet, and cut into four 7.62 cm × 4.45 cm square pieces. This process minimizes air bubbles or poor compaction in theclay witness. The molded clay block was held onto the back of the target using a strip of adhesive tape.In order to normalize results with respect to variations in impact velocities, ballistic test results are also presented in terms ofdissipated projectile kinetic 5
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012 schematic diagram of ballistic experimental setup. where E is the dissipated energy (J), mp is the projectile mass (kg), Vi is the initial projectile velocity (m/s), and Vr is the residual velocity of the projectile after penetrating the target (m/s).In order to relate depth of penetration to residual projectile velocity, a series of experiments were performed using an empty target frame and clay witness resulting penetration depth as a function of projectile velocity, which is closely modeled by the linear relationship Vr = 38.9 + 3720 L Where L (m) is the penetration depth into the clay witness. Equations 1 and 2 are used throughout this paper to relate depth of penetration to residual projectile kinetic energy. The energy dissipated by the target is normalized by the initial kinetic energy of the projectile to obtain the fractional dissipation. Velocity, V (m/s)Penetration Depth, L (m)8.2 Flexibility and thickness testsTwo-dimensional drape tests were performed tomeasure the flexibility of the targets, in all cases a 20 gweight was used, and encapsulated ballistic targets wereused as the test specimens. Bending angle is reported asa measure of target flexibility, with larger anglesindicating greater flexibility. Target thickness at thecenter of the targets was also measured with amicrometer. 8.3 Results Rheological properties of shearthickening suspension The steady shear viscosity as a function of the steadyshear rate for the ethylene glycol based silica suspensionat volume fractions of φ = 0.57 and 0.62. Note that thedata are collected on a controlled stress remoter wherean applied shear stress is controlled and thecorresponding shear rates measured. However, the datahas been plotted against the measured shear rate ratherthan the applied stress, as is more traditional. The use ofcontrolled stress enables probing the regime of extremeshear thickening observed at high shear rates, which isnot possible in a controlled rate device due to the natureof the material’s response. Both shear thinning and shear thickening behavior are observed. At these high particle loadings,the silica suspensions are glassy at rest and yield at low shear rates. This manifests in Fig. 7 as strong shear thinning η( ˙ γ)∝ ˙ γ −1, which is a signature of a yield stress th increasing shear rate the viscosity begins to plateau, followed by atransition to shear thickening behavior at high shear rates. The shear thickening transition was observed to occur at shearrate of 10 s−1 for the concentrated dispersion having a particle volume fraction of φ = 0.62 and 300 s−1 for the fluid with aparticle volume fraction of φ = 0.57. At high shear rates in the shear thickening region, the high volume fraction (φ =0.62)dispersion exhibits a greater increase in viscosity. Transducer limitations and sample adhesive failure to the tooling silicadispersed in ethylene glycol for steady shear flow. prevented exploration of higher shear stresses. However, careful analysisof the slip in these materials [20, 25] demonstrates that the sample solidifies in the shear thickened regime, such that thereported viscosities. 6
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012 After the onset of shear thickening are more representative of the suspension slipping against the tooling. Note also that the shear thickening transition is reversible, i.e., this liquid-to-solid transition induced by flow is not associated with particle aggregation, nor it results in any irreversible change in the dispersion. This effect is shown in as the data plotted corresponds to both ascending and descending shear stresses without hysteresis. The shear thickening transition in colloidal dispersions is believed to result from a micro structural change where the hydrodynamic forces overcome antiparticle forces to create particle clusters . These cluster formations, referred to as “hydro clusters,” increase the hydrodynamic stress in the suspension, thus marking the onset of shear thickening. The hydro clustered state, however, does not lead to permanent or irreversible particle aggregation. Additional rheological studies have shown that the timescales for this transition are on the order of millisecond or less [15, 20, 25].The characteristic shear rate for the ballistic testing performed here is estimated to be on the order of 45,000 1/s ( ˙ γ = vx/y = 24400/0.56), based on a projectile velocity of 800 fps (244 m/s) and a projectile diameter of 22 caliber (0.56 cm). This shear rate greatly exceeds the rate required for the onset of shear thickening in this fluid (about 300 1/s for the silica suspension with φ = 0.57). Thus we expect the shear ratesduring the ballistic tests to be sufficient to transition the dispersion to its shear thickened state.8.4 Ballistic test resultsThe ballistic test results of a series of targets composed of 4layers of Kevlar and 8 ml of STF with different configurations(targets A to F in Fig. 8) are shown in Figs 9–11 andsummarized in Table I. The projectile has been stopped in alltargets. Fig. 9 shows the energy dissipation for these targets,with the fully impregnated targets (E, F) showing significantlyless penetration depth than the unimpregnated targets (A, B, C,D). The clay witness penetration profiles (Fig. 10) also show amarked difference in shape, as the unimpregnated targets show sharp, deep penetration profiles, while the impregnatedsamples show a blunt, shallow impregnation. These results clearly show that impregnating the STF into the fabric is criticalto achieving an enhancement in the fabric ballistic properties. Shows the front Kevlar layers for targets D(Unimpregnated)and F (impregnated). The unimpregnated target shows that the Kevlar yarns that were directly impacted by the projectilepullout significantly from the weave, producing the well-documented cross pattern in the fabric.Note that the Kevlar layers exhibit little actual fiber breakage, although some fiber stretching near the impact point mayhave occurred. In contrast, the first layer of Kevlar in the impregnated target shows extensive fiber breakage near theprojectilecontact point, and only very little yarn pullout or wrinkling in the surrounding fabric. Some fiber stretching may haveoccurred at the impact point. Note that yarn pullout is evident only for the yarns directly impacted by the projectile, with thetotal pullout distance significantly less than that observed for the neat Kevlar target. Having demonstrated that fabricimpregnation is essential to realizing enhanced performance; further targets were constructed to establish the scaling ofenergy absorption with the relative amount of STF and Kevlar in the target. Table II and Fig. 12 show the energy dissipatedby targets consisting of 4 impregnated layers ofFabric, as a function of the volume of STF. As shown in this figure, the energy absorption by the target increasescontinuously with the total volume of STF in the target. To demonstrate that the enhanced ballistic performance of theimpregnated fabrics is not simply a consequence of increased target mass or solvent effects on the Kevlar weave tests wereperformed using Kevlar that was impregnated with pure ethylene glycol. As shown in Fig. 12, samples of ethylene glycol-impregnated Kevlar show relatively poor ballistic performance compared with STF-impregnated Kevlar with equalimpregnated fluid volume. In this graph, the dotted line shows the amount of energy dissipated by 4 layers of pure Kevlar 7
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012(target G). The results show that the addition of ethylene glycol does not improve the impact energy absorption capacity ofKevlar fabric. In fact, at high loadings (8 ml ethylene glycol) the performance is even worse than neat Kevlar, despite theincreased target mass. This decrease in performance may be due to lubrication effects, as the solvent (which is Newtonian atthese shear rates, unlike the shear thickening fluid) may reduce the friction between fibers in the fabric during yarn pullout.A direct comparison between the ballistic protection performance of targets consisting of pure Kevlar fabric and STF-impregnated Kevlar fabric with nearly equal total weight hasbeen made in Table III and Fig. 13. As shown in Fig. 13, thecomposite, impregnated targets have the same ballisticresistance as targets of equal than the number of Kevlar layersin the neat Kevlar targets.8.5 Flexibility and thickness test resultsThe test results for the flexibility of 4 layers of Kevlar, 10layers of Kevlar and 4 layers of Kevlar impregnated with 2 mlSTF are presented in Table IV. The weight and ballisticperformance of the 4-layer STF impregnated Kevlar is nearlythe same as that of the10-layer unimpregnated Kevlar.However, the 4-layer STF-impregnated Kevlar is moreflexible (bending angle = 51◦) than the 10-layerunimpregnated Kevlar (bending angle = 13◦) with sameoverall weight. In fact, there is no difference in flexibilitybetween them . 9. DiscussionThe results clearly demonstrate that, under our test conditions,impregnating neat Kevlar fabric with STF enhances theballistic properties of the fabric. More precisely, the additionof STF to the fabric increases the amount of projectile energythat is absorbed by the target. A number of possible mechanisms could explain this behavior. Fig. 11 shows that theimpregnated fabric exhibits significantly less pullout that the unimpregnated fabric, both in terms of the number of yarnspulled and the pullout distance per yarn. The impregnated target, unlike the neat fabric, also exhibits significant fiberfracture at the impact point. Anotherimportant difference is that all four layers of fabric in target D (not shown) exhibitedextensive pullout, comparable to that of the first layer of fabric. In contrast, the three backing layers of target F (not shown)exhibited little or no pullout, and no fiber fracture. Therefore, most of the energy absorption in the impregnated target waslikely provided by the first layer of Kevlar, although the backing layers may still have provided a critical secondary roleduring the impact event. These results suggest that the STF constrains the Kevlar yarns as they are pulled through the fabric.The increase in energy dissipation in the impregnated target could be due in part to an increase in force required to pullouteach yarn from the fabric, so that less totalpullout is required to absorb the projectile energy. An alternative explanation isthat the increased pullout resistance increases the loads on the yarns during impact which then absorb additional energythrough fiber deformation and fracture. To address these issues, we are performing additional ballistic tests at highervelocities, and performing quasistatic yarn pullout tests [3,27] with and without STF.10. Conclusions and future workThis study demonstrates that the ballistic penetration resistance of Kevlar fabric is enhanced by impregnation of the fabricwith a colloidal shear thickening fluid. Impregnated STF-fabric composites are shown to provide superior ballisticprotection as compared with simple stacks of neat fabric and STF. Comparisons with fabrics impregnated with non-shearthickening fluids show that the shear thickening effect is critical to achieving enhanced performance. Energy absorption bythe STF-fabric composite is found to be proportional to the volume of STF. Compared with neat Kevlar fabrics ofequivalent weight, the STF-impregnated Kevlar fabric provides nearly the same ballistic protection, yet is much thinner andmore flexible. 8
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012ReferencesAusiello, P., Apicella, A., Davidson, C. L. (2002). Effect of adhesive layer on stressdistribution in composite restorations – a 3D finite element analysis, DentalMaterials, 18, 295-303.Beckert, W., Lauke, B. (1995). Fracture mechanics finite element analysis of debonding crackextension for a single fibre pull-out specimen, J. Mat. Sci. Lett., 14, 333-336.Boisse, P., Borr, M., Buet, K., Cherouat, A. (1997). Finite element simulations of textilecomposite formed including the biaxial fabric behavior, Comp. B, Eng., 28, 453-464.Butcher, R. J., Rousseau, C. E., Tippur, H. V. (1999). A functionally graded particulatecomposite: Preparation, Measurements and failure analysis, Acta Mater. 47, 259-268.Chang, F. K., Scott, R. A., Springer, G. S. (1982). Strength of mechanically fastened compositejoints, J. Comp. Mat. 16, 470-494.Change, F. K., Chang, K. Y. (1987). A progressive damage model for laminated compositescontaining stress concentrations, J. Comp. Mat., 21, 834-855.Chen, X., Liu, Y. (2001). Multiple-cell modelling of fibre-reinforced composites with thepresence of interphases using the boundary element method, Comp. Mat. Sci. 21,86-94.Choo, H., Bourke, M. A. M., Daymond, M. R. (2001). A finite-element analysis of the inelasticrelaxation of thermal residual stress in continuous-fiber-reinforced composites,Comp. Sci. Tech., 61, 1757-1722.Davies, G. A. O., Zhang, X., Zhou, G., Watson, S. (1994). Numerical modelling of impactdamage, Composites, 25, 342-350.Dehoff, P. H., Anusavice, W. J., Wang, Z. (1995). Three-dimensional finite element analysisof the shear bond test, Dent. Mater., 11, 126-31.Diaz, J., Romera, L., Hernandez, S., Baldomir, A. (2010). Benchmarking of three-dimensionalfinite element models of CFRP single-lap bonded joints, Int. J. Adhesion andAdhesives, 30, 178-189.312 Finite Element AnalysisDooms, D., Degrande, G., Roeck, G. D., Reynders, E. (2006). Finite element modelling of asilo based experimental nodal analysis, Eng. Structures, 28, 532-542.Fisher, F. T., Bradshaw, R. D., Brinson, L. C. (2003). Fiber waviness in nanotube-reinforcedpolymer composites—II: modeling via numerical approximation of the dilute strainconcentration tensor, Comp. Sci. Tech., 63, 1705-1722.Fisher, F. T., Brinson, L. C. (2001). Viscoelastic interphases in polymer-matrix composites:Theoretical models and finite element analysis, Composites Sci. and Tech. 61,731-748.Gamble, K., Pilling, M., Wilson, A. (1995). An automated finite element analysis of theinitiation and growth of damage in carbon-fibre composite materials, Comp.Structures, 32, 265-274.Guild, F. J., Young, R. J. (1989). A predictive model for particulate-filled composite materials,J. Mat. Sci., 24, 298-306.Houshyar, S., Hodzic, A., Shanks, R. A. (2009). Modelling of polypropylene fibre-matrixcomposites using finite element analysis, eXPRESS Polymer Letters, 3, 2-12.Houshyar, S., Shanks, R. A. (2003). Morphology, thermal and mechanical properties ofpoly(propylene) fibre-matrix composites, Macromol. Mat. Eng., 288, 599-606.Houshyar, S., Shanks, R. A. (2010). Interfacial properties of all-polypropylene composites, e-Polymers, 33, 1-13.Houshyar, S., Shanks, R. A., Hodzic, A. (2005). The effect of fiber concentration onmechanical and thermal properties of fiber-reinforced polypropylene composites, J.Appl. Polym. Sci., 96, 2260-2272.Huang A., Bush M. B. (1997). Finite element analysis of mechanical properties indiscontinuously reinforced metal matrix composites with ultra fine micro structure.Mat. Sci. Eng. A, 232, 63–72. 9
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.2, 2012Hutchinson, J. W., Jensen, H. M. (1990). Models of fiber debonding and pullout in brittlecomposites with friction, Mecahnical of Materials, 9,139-163.Hyung, Y. C., Wu, H. Y. T., Fu-Kuo, C. (1991). A new approach toward understandingdamage mechanisms and mechanics of laminated composites due to low-velocityimpact. II: analysis, J. Comp. Mat., 25, 1012-1038.Isakson, G., Levy, A. (1971). Finite element analysis of interlaminar shear in fibrouscomposites, J. Comp. Mat., 5, 273-276.Kang G. Z., Gao Q. (2002). Tensile properties of randomly oriented short Al2O3 fibrereinforced aluminium alloy composites: II. Finite element analysis for stresstransfer, elastic modulus and stress-strain curve. Composites A, Appl. Sci.Manufacturing, 33, 657–667.Lamkanfi, E., Paepegem, W. V., Degrieck, J., Ramault C. (2010). Strain distribution incruciform speciments subjected to biaxial loading conditions. Part 1. Twodimensionalfinite element model, Polym. Testing, 29, 7-13.Lee, S. H., Wang, S., Pharr, G. M., Xu, H. (2007). Evaluation of interphase properties in acellulose fiber-reinforced polypropylene composite by nanoindentation and finiteelement analysis, Composites A, 38, 1517-1524.Lim, J. H., Ratnam, M. M., Abdul-Khalil H. P. S (2003). An experimental and finite elementanalysis of the static deformation of natural fiber-reinforced composite beam,Polym. Testing, 22, 169-177.Modelling of polymeric fibre-composites and finite element simulation of mechanical properties 313Lin, D. X., Ni, R. G., Adams, R. D. (1984). Prediction and measurement of the vibrationaldamping parameers of carbon and glass fire-reinforced plastics plates, J. Comp.Mat., 18, 132-152.McCarthy, M. A., McCarthy, C. T. (2002). Finite element analysis of the effects of clearanceon single-shear, composite bolted joints, J. Plastics, Rubber Comp., 32, 1-11.Maligno A. R., Warrior N. A., Long A. C. (2008). Finite element investigations on themicrostructure of fibre reinforced composites. Express Polymer Letters, 2, 665–676.Muheim, D., Griffen, O. H. (1990). 2-D to 3-D global/local finite element analysis of crossplycomposite laminates, J. Reinforced Plastics Comp., 9, 492-502.Naik, N. K., Shembekar, P. S. (1992). Elastic behaviour of woven fabric composites: I –lamina analysis, J. Comp. Mat.,26, 2196-2225.Nakamura, T., Imanishi, A., Kashima, H., Ohyama, T., Ishigaki, S. (2001), Stress analysis ofmetal-free polymer crowns using the three-dimensional finite element method, Int.J. Prosthodont, 14, 401-405.Nedele, M. R., Wisdom, M. R. (1994). Three-dimensional finite element analysis of the stressconcentration at a single break, Comp. Sci. Tech., 51, 517-524.Pal, P., Ray, C. (2002). Progressive failure analysis of laminated composite plates by finiteelement method, J. Reiforced Plastics and Composites, 21, 1505-1513.Pavier, M. J., Clarke, M. P. (1996). Finite element prediction of the post-impact compressivestrength of fibre composites, Comp. Structures, 36, 141-153.Pegoretti, A., Fambri, L., Zappini, G., Bianchetti, M. (2002). Finite element analysis of a glassfibre reinforced composite endoplastic post, Biomaterials, 23, 2667-2682.Shati F. K., Esat I. I., Bahai H. (2001). FEA modelling of visco-plastic behaviour of metalmatrix composites. Finite Elements in Analysis and Design, 37, 263–272.Song, Y. S., Youn, J. R. (2006). Evaluation of the effective thermal conductivity for carbonnanotube/polymer composites using control volume finite element method,Carbon, 44,710-717.Soykasap, O. (2010). Finite element analysis of plain weave composites for flexural failure,Polym. Composites, 31, 581-586.Sun, C. T., Chen, J. K. (1985). On the impact of initially stressed composite laminates, J.Comp. Mat., 19, 490-504.Tan, P., Tong, L., Steven, G. P. (1998). Modelling approaches for 3D orthogonal wovencomposites, J. Reinforced Plastics Comp., 17, 545-577. 10
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. Prospective authors ofIISTE journals can find the submission instruction on the following page:http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar